Carbohydrate Polymers 90 (2012) 413–418
Contents lists available at SciVerse ScienceDirect
Carbohydrate Polymers journal homepage: www.elsevier.com/locate/carbpol
Bacterial cellulose/silica nanocomposites: Preparation and characterization Alireza Ashori a,∗ , Somayeh Sheykhnazari b , Taghi Tabarsa b , Alireza Shakeri c , Masood Golalipour d a
Department of Chemical Technologies, Iranian Research Organization for Science and Technology (IROST), P.O. Box 15815-3538, Tehran, Iran Department of Wood and Paper Technology, Gorgan University of Agricultural Sciences & Natural Resources, Gorgan, Iran c Department of Chemistry, University of Golestan, Gorgan, Iran d Department of Biology, University of Golestan, Gorgan, Iran b
a r t i c l e
i n f o
Article history: Received 6 March 2012 Received in revised form 16 May 2012 Accepted 19 May 2012 Available online 27 May 2012 Keywords: Bacterial cellulose Tetraethoxysilane (TEOS) Nanocomposite Young’s modulus FE-SEM
a b s t r a c t The preparation and characterization of bacterial cellulose (BC)/silica nanocomposites are presented in this paper. BC hydro-gel was immersed in an aqueous solution of tetraethoxysilane (TEOS). By pressing the treated BC matrices at 120 ◦ C and 2 MPa, water-free translucent sheets were obtained. TEOS concentration (3, 5 and 7%) and press time (8, 10 and 12 min) were used as variable factors. These materials were characterized by different techniques, namely FE-SEM, FTIR, SEM, tensile strength and Young’s modulus. All composites showed good dispersion of the ﬁbers and strong adhesion between the ﬁbers and the matrix. FE-SEM observations showed that the nano-scale silica was embedded between the voids and micro-ﬁbrils of the BC matrix. Reﬂecting this structure, the maximum Young’s modulus and tensile strength of dry BC/silica composites improved to 1.46 GPa and 113 MPa, respectively. The tensile strength and Young’s modulus showed 35 and 18-fold increase (with 7% TEOS), respectively, while the same properties were reduced 15 and 10-fold with increase in press time from 8 to 12 min. FTIR results illustrated strong chemical interactions between the cellulose and silica phases. The optimum condition was obtained when the TEOS dosage and press time were 7% and 8 min, respectively. © 2012 Elsevier Ltd. All rights reserved.
1. Introduction Today, due to the global demand for ﬁbrous materials, worldwide shortage of wood biomass in many areas, and environmental awareness, bacterial cellulose (BC) has become one of the promising alternative sources of ﬁbrous materials for the 21st century (Sun, Yang, & Wang, 2010; Wan et al., 2009). In recent years, a great deal of interest has been generated for the production of cellulose using biotechnology method, which reduces the environmental impact to a minimum. Studies suggest that BC may be a better choice for manufacturing cellulose products (Castro et al., 2011; Czaja, Romanovicz, & Malcolm Brown, 2004), since BC is produced in a pure (free of impurities such as lignin and extractives) and crystalline form, which makes its recovery relatively simple. In terms of chemical structure, BC is identical to that produced by plants. However, it exhibits higher crystallinity, water-holding capacity, degree of polymerization, and mechanical strength (Darder, Aranda, & Ruiz-Hitzky, 2007; Sheykhnazari, Tabarsa, Ashori, Shakeri, & Golalipour, 2011). These properties make BC an interesting biomaterial for applications as nutritional component (Sani & Dahman, 2010), artiﬁcial skin (Hungund & Gupta, 2010), ﬂexible display screens (Nakagaito, Nogi, & Yano,
∗ Corresponding author. Tel.: +98 21 5627 6637; fax: +98 21 5627 6265. E-mail address: [email protected]
(A. Ashori). 0144-8617/$ – see front matter © 2012 Elsevier Ltd. All rights reserved. http://dx.doi.org/10.1016/j.carbpol.2012.05.060
2010), and in traditional applications where plant cellulose is used (Castro et al., 2011). Historically, plant derived cellulose has been used either as reinforcement (Ashori & Nourbakhsh, 2010; Mottershead & Eichhorn, 2007; Nourbakhsh, Karegarfard, Ashori, & Nourbakhsh, 2010) or matrix (Darder et al., 2007), or as the sole component to prepare all-cellulose composites (Soykeabkaew, Arimoto, Nishino, & Peijs, 2008). Recently, BC has been used as reinforcement for various composites due to its excellent mechanical performance (Ifuku et al., 2007; Nakagaito, Iwamoto, & Yano, 2005; Sun et al., 2010). For instance, Gindl and Keckes (2004) prepared cellulose acetate butyrate based composites reinforced with BC sheets. Yano et al. (2005) demonstrated the production of nanocomposites made with BC nanoﬁbers and acrylic resin. High-strength BC/phenolic resin composites were produced by Nakagaito et al. (2005). Hu et al. (2009) evaluated the bacterial cellulose nanoﬁber-reinforced unsaturated polyester resin composites. Nanoﬁbers and nanocomposite materials have gained much interest due to their remarkable change in properties. These materials can be combined effectively to obtain a new class of high performance or highly functional organic–inorganic hybrid materials. In recent years, cellulose-based nanocomposites have deﬁnitely proved their exceptional potential by providing a possibility of synthesizing a signiﬁcant number of new nanomaterials with high degree of homogeneity and purity at molecular level and with extraordinary physical and chemical properties (Xie, Yu, & Shi,
A. Ashori et al. / Carbohydrate Polymers 90 (2012) 413–418 Table 1 Two variable factors and their combinations used in this study.
Fig. 1. Schematic model of cellulose/silica covalent crosslinking materials (Xie, Yu, et al., 2009).
2009). The reaction process involves the hydrolysis of silica precursors and condensation of the resulting hydroxyl groups to form a nanostructure. One simple method is mixing organic compounds with a metal alkoxide, such as tetraethoxysilane (TEOS). During the process, the inorganic mineral is deposited in the organic compound matrix forming hydrogen bonding between the organic and inorganic phases (Fig. 1). The BC ﬁber is one of the excellent natural biomaterials. BC has been explored as a substrate for composite materials because of the presence of several functional groups that may be employed in various activation processes. Chemical modiﬁcation of BC can change its chemical and morphological structures for different purposes (Hou, Wang, & Yu, 2009; Xie, Zhang, & Yu, 2009). The present study describes the preparation and characterization of nanocomposite materials obtained using BC and silica. In addition, the effects of TEOS and press time on the morphological and mechanical properties of BC-based nanocomposites have been investigated.
Press time (min)
8 10 12 8 10 12 8 10 12
3 3 3 5 5 5 7 7 7
A1 A2 A3 B1 B2 B3 C1 C2 C3
(Sheykhnazari et al., 2011). In brief, G. xylinus was incubated in a static Hestrin–Schramm culture at 28 ◦ C for 14 days. The obtained gel-like BC pellicles, about 6-mm thick, were puriﬁed by immersion in deionized water at 90 ◦ C for 2 h and then boiled in a 0.5 M aqueous solution of NaOH for 15 min. The BC pellicles were then washed with deionized water several times and soaked in 1% NaOH for 2 days. Subsequently, the BC pellicles were washed free of alkali. Finally, a tridimensional network of nano- and micro-ﬁbrils of BC with 10–100 nm width was obtained. TEOS was used as a precursor. It was an analytical grade from Merk Co., Germany. 2.2. Preparation of BC/silica nanocomposites
2. Materials and methods
The BC/silica composite samples were prepared by the solution impregnation method. A certain amount of TEOS was mixed with 100 g of water together with 0.5 mL acetic acid (0.1N), and the mixture was stirred for 1 h. In order to control the silica content in BC gel, TEOS concentration in water was varied, i.e. 3, 5, 7%. BC gels were immersed in the TEOS solution and allowed to stand for 2 days. At high concentration of TEOS, brittle BC/silica mats were obtained. Subsequently, all surfaces of samples were wiped off with a dry cloth. Dry translucent BC/silica sheets were obtained by pressing BC/silica mats at 120 ◦ C and 2 MPa. The process of preparation of the BC/silica composite is shown in Fig. 2. Experimental schedule is shown in Table 1. As it can be seen, the two variable factors were TEOS concentration and press time.
2.3. Sample characterization
The organism used was Gluconacetobacter xylinus (BPR 2004), which was obtained from the DSMZ Laboratory, Germany. The preparation procedures of BC were reported elsewhere
The particle size of silica was investigated by a ﬁeld emission-scanning electron microscope (FE-SEM, Hitachi 4160) with an accelerating potential of 15 kV. Scanning electron
Fig. 2. Preparation process of dry and pressed BC/silica sheets from BC gels (Maeda et al., 2006).
A. Ashori et al. / Carbohydrate Polymers 90 (2012) 413–418
microscopy (SEM) was used to observe the microorganism morphology and its distribution in the composite. A CamScan MV2300 SEM operating at 15 kV was used. Before scanning, each sample was coated with gold to improve its interface conductivity. 2.4. Fourier transform infrared spectroscopy (FTIR) FTIR spectroscopy was used primarily to identify the chemical structure of the BC and BC/silica composites. Infrared absorption spectra were obtained from 4000 to 400 cm−1 using KBr pellets in a PerkinElmer spectrometer, model 2000. 2.5. Mechanical testing Test specimens of 30 mm length and 10 mm width were cut from composite sheets. All specimens were equilibrated in a chamber kept at 20 ◦ C and 35% relative humidity for 24 h before testing. The tensile strength of the plain matrix and all composites was measured by employing ASNTM STM universal tensile machine following ASTM D 5937-1996. The crosshead speed was set at 5 mm/min. All tests were conducted at ambient temperature and an average value of four repeated tests was taken for each treatment. 2.6. Statistical analysis The experimental design consisted of two treatments (including TEOS concentration and press time) and their interactions. Data for each treatment was statistically studied by analysis of variance (ANOVA). When the ANOVA indicated a signiﬁcant difference among factors and levels, a comparison of the means was done, employing Duncan’s multiple range test (DMRT), to identify the groups that were signiﬁcantly different from other groups at 99% and 95% conﬁdence levels.
Fig. 3. SEM images of (a) BC micro-ﬁbrils and (b) BC/silica composite.
3. Results and discussion 3.1. Microstructure A set of selected SEM micrographs of the surface of BC and BC/silica composite materials was studied. Representative SEM micrographs are shown in Fig. 3. For each material, the BC ﬁbers dispersion and the interfacial adhesion are shown. Obviously, in the case of BC, only the small mat fragments, and not the isolated ﬁbrils, were observed (Fig. 3a). Fig. 3b shows the surface of pressed and dried BC/silica sheets. The SEM micrographs provided evidence of the strong interfacial adhesion between the BC ﬁbers and the matrix, as shown by the good dispersion within the matrix, without noticeable aggregates. As mentioned before, BC gel was immersed into aqueous solution of TEOS and silica was ﬁnally deposited on BC micro-ﬁbrils via silanol. It is known that silanol is reactive and reacts with hydroxyl groups on organic polymers such as poly(vinyl alcohol), or polydimethylsiloxane having hydroxyl groups on both chain ends in organic–inorganic hybrids (cited by Maeda, Nakajima, Hagiwara, Sawaguchi, & Yano, 2006). Therefore, BC micro-ﬁbrils having free hydroxyl groups may undergo condensation reactions with supplied silanol, which becomes ﬁxed to micro-ﬁbrils. Silanol itself also condenses forming silica, and is deposited on BC microﬁbrils through hydrogen bonding or condensation reactions with cellulose. These results clearly corroborated the superior mechanical properties of the BC/silica composites compared with BC
material, as suggested by the mechanical tests discussed by Maeda et al. (2006). FE-SEM analysis of the BC/silica composites was used to characterize the distribution of silica particles on the BC micro-ﬁbrils (Fig. 4a) and the particle size of silica (Fig. 4b). Fig. 4a shows that there were a lot of silica particles on the composites surface. As mentioned earlier, BC was immersed in a silanol sol prepared from TEOS dispersed in water using acetic acid as a catalyst. Silica particles were deposited on the spaces/voids between BC nano- and micro-ﬁbrils.
3.2. FTIR spectroscopy Table 2 summarizes all FTIR results for BC, amorphous silica and BC/silica composites. Fig. 5 shows FTIR spectra obtained from three representatives BC/silica composites including A1, B1 and C1. As it can be seen in Table 2, there are some differences between the BC and BC/silica FTIR results that may be related to the strong chemical interactions between the cellulose and silica phases. The important changes among the spectra presented in Fig. 5a–c can be assigned to: 3200–3700 cm−1 (Si OH), 1110–830 cm−1 (Si O), and 460 cm−1 (Si O Si). This result is in good agreement with the works previously reported by Barud et al. (2008) and De Salvi, Barud, Caiut, Messaddeq, and Ribeiro (2012).
A. Ashori et al. / Carbohydrate Polymers 90 (2012) 413–418
Fig. 5. FTIR spectra: (a) BC/silica 3%, (b) BC/silica 5% and (c) BC/silica 7%.
3.3. Mechanical properties Fig. 4. FE-SEM micrographs (a) distribution of silica particles on the BC micro-ﬁbrils and (b) nanoparticles of silica.
Table 2 FTIR results for BC, silica and BC/silica nanocomposite. Assignment
Wavenumber (cm−1 ) BC
O H bending b-Glucosidic linkages between the glucose units C O symmetric stretching of primary alcohol C O C antisymmetric bridge stretching C H deformation CH2 bending or O H in plane bending H O H bending of absorbed water CH2 CH stretching of CH2 and CH3 groups H-bond OH stretching Si O Si bending Si O Si symmetric stretching Si OH stretching Si O stretching Water OH bending Water and silanol OH stretching OH stretching C H stretching Water OH bending CH2 bending C O C bond O H out-of-phase bending Si O Si bending
400–700 ∼896 1040 1168 1340 1400 1650 2700 2900 3246 3500 462 804 949 1110 1640 3460 3300 2900 1640 1400 1160 600 460
The most crucial factor that affects the mechanical properties of the composite materials is the ﬁber matrix interfacial adhesion. The quality of interfacial bonding is determined by several factors, such as the nature of ﬁller and polymer components, the ﬁber aspect ratio, the processing procedure and the ﬁller treatment (Nourbakhsh et al., 2010). Statistical analysis showed that the mechanical properties in terms of tensile strength and Young’s modulus of the samples were signiﬁcantly inﬂuenced by the TEOS concentration and press time (Table 3). However, the interaction of variable factors was not signiﬁcant. According to the DMRT, the differences between the mean values of the studied properties within and among each of the groups compared, were signiﬁcant. For easier comparison between the mechanical performances of the various composites, the results are presented in Fig. 6. As clearly seen, all samples (group C) made with 7% TEOS had the highest values among the other types of specimens. In addition, both mechanical properties were decreased when the press time was increased from 8 to 12 min. With increase in press time, more heat can be transferred to the sheet, which would degrade the crosslinking between BC and TEOS. In addition, an increasing trend in tensile properties with silica content is found from Fig. 6. The superior mechanical properties of composites ﬁlled with 7% TEOS compared with those ﬁlled with 3 and 5% TEOS, conﬁrmed the good interfacial adhesion and the strong interactions between the silica and the BC matrix. It is well accepted that tensile strength and Young’s modulus of composites are inﬂuenced by the nature of matrix and the adhesion between ﬁber and matrix. Similar results have been reported by Xie, Yu, and Shi (2009) who studied the properties of cellulose/silica hybrid nanocomposites. Their data showed that the incorporation of nanoscale particles into cellulose matrix leads to a strong interfacial interaction.
A. Ashori et al. / Carbohydrate Polymers 90 (2012) 413–418
Table 3 Results of ANOVA test on the effect of variables and their interaction on the mechanical properties. Source of variations
A B A×B Error Total
2 2 4 18 26
4571.97 1159.04 9.20 848.41 6587.62
2285.98 579.02 2.3 47.14
48.5** 12.28** 0.049ns
0.233845 0.047639 0.007533 0.070755 0.359773
0.117 0.024 0.002 0.003931
29.745** 6.06* 0.479ns
Note: A = TEOS concentration; B = press time; df = degree of freedom; MS = mean of squares; SS = sum of squares; F = F value; ns = not signiﬁcant. ** Signiﬁcant difference at the 1% level (p ≤ 0.01%). * Signiﬁcant difference at the 5% level (p ≤ 0.05%).
120 Young's modulus Tensile strength
Tensile strength (MPa)
Young's modulus (GPa)
Treatment codes Fig. 6. Effects of TEOS concentration and press time on the mechanical properties.
4. Conclusions The morphological and mechanical properties of BC/silica composites were evaluated to determine the inﬂuences of TEOS concentration (3, 5 and 7%) and press time (8, 10 and 12 min). Some conclusions are as follows: a) In the present study, BC gel was immersed into aqueous solution of TEOS and silica was ﬁnally deposited on BC micro-ﬁbrils via silanol. b) The scanning micrographs provided evidence of the strong interfacial adhesion between the BC ﬁbers and the matrix, as shown by the good dispersion within the matrix, without noticeable aggregates. This was attributed to the chemical bonding on the ﬁber–matrix interface under the function of TEOS coupling agent. c) A decrease in both mechanical properties is observed for all composites when press time is increased from 8 to 12 min. d) The tensile strength and Young’s modulus increased by 35 and 18 fold (with 7% TEOS), while the same properties showed 15 and 10 fold reduction with increase in press time from 8 to 12 min, respectively. e) Among the various formulations, composites C1 (7% TEOS and 8 min press time) had the maximum improvement in both mechanical properties. f) FTIR spectra showed some differences between the BC and BC/silica samples, which is related to the chemical interactions between the cellulose and silica phases. g) Finally, it was found that deposited nanoparticles of silica between BC nano- and micro-ﬁbrils reinforced the composite. References Ashori, A., & Nourbakhsh, A. (2010). Reinforced polypropylene composites: Effects of chemical compositions and particle size. Bioresource Technology, 101(7), 2515–2519.
Barud, H. S., Assunc¸ão, R. M. N., Martines, M. A. U., Dexpert-Ghys, J., Marques, R. F. C., Messaddeq, Y., et al. (2008). Bacterial cellulose–silica organic–inorganic hybrids. Journal of Sol–Gel Science and Technology, 46(3), 363–367. ˜ Castro, C., Zuluaga, R., Putaux, J.-L., Caro, G., Mondragon, I., & Ganán, P. (2011). Structural characterization of bacterial cellulose produced by Gluconacetobacter swingsii sp. from Colombian agroindustrial wastes. Carbohydrate Polymers, 84(1), 96–102. Czaja, W., Romanovicz, D., & Malcolm Brown, R. (2004). Structural investigation of microbial cellulose produced in stationary and agitated culture. Journal of Cellulose, 11(3–4), 403–411. Darder, M., Aranda, P., & Ruiz-Hitzky, E. (2007). Bionanocomposites: A new concept of ecological, bioinspired, and functional hybrid materials. Advanced Materials, 19(10), 1309–1319. De Salvi, D. T. B., Barud, H. S., Caiut, J. A., Messaddeq, Y., & Ribeiro, S. J. L. (2012). Selfsupported bacterial cellulose/boehmite organic–inorganic hybrid ﬁlms. Journal of Sol–Gel Science and Technology, http://dx.doi.org/10.1007/s10971-0071669-9 Gindl, W., & Keckes, J. (2004). Tensile properties of cellulose acetate butyrate composites reinforced with bacterial cellulose. Composites Science and Technology, 64(15), 2407–2413. Hou, A., Wang, X., & Yu, Y. (2009). Preparation of the cellulose/silica hybrid containing cationic groups by sol–gel crosslinking process and its dyeing properties. Carbohydrate Polymers, 77(2), 201–205. Hu, L., Wan, Y., He, F., Luo, H. L., Liang, H., Li, X., et al. (2009). Effect of coupling treatment on mechanical properties of bacterial cellulose nanoﬁbre-reinforced UPR ecocomposites. Materials Letters, 63(22), 1952–1954. Hungund, B. S., & Gupta, S. G. (2010). Strain improvement of Gluconacetobacter xylinus NCIM 2526 for bacterial cellulose production. African Journal of Biotechnology, 9(32), 5170–5172. Ifuku, S., Nogi, M., Abe, K., Handa, K., Nakatsubo, F., & Yano, H. (2007). Surface modiﬁcation of bacterial cellulose nanoﬁbers for property enhancement of optically transparent composites: Dependence on acetyl-group DS. Biomacromolecules, 8(6), 1973–1978. Maeda, H., Nakajima, M., Hagiwara, T., Sawaguchi, T., & Yano, S. (2006). Bacterial cellulose/silica hybrid fabricated by mimicking biocomposites. Journal of Materials Science, 41(17), 5646–5656. Mottershead, B., & Eichhorn, S. J. (2007). Deformation micromechanics of model regenerated cellulose ﬁbre–epoxy/polyester composites. Composites Science and Technology, 67(10), 2150–2159. Nakagaito, A. N., Iwamoto, S., & Yano, H. (2005). Bacterial cellulose: The ultimate nano-scalar cellulose morphology for the production of high-strength composites. Applied Physics A, 80, 93–97. Nakagaito, A. N., Nogi, M., & Yano, H. (2010). Displays from transparent ﬁlms of natural nanoﬁbers. MRS Bulletin, 35(3), 214–218. Nourbakhsh, A., Karegarfard, A., Ashori, A., & Nourbakhsh, A. (2010). Effects of particle size and coupling agent on mechanical properties of particle-reinforced composites. Thermoplastic Composite Materials, 23(2), 169–174.
A. Ashori et al. / Carbohydrate Polymers 90 (2012) 413–418
Sani, A., & Dahman, Y. (2010). Improvements in the production of bacterial synthesized biocellulose nanoﬁbres using different culture methods. Journal of Chemical Technology and Biotechnology, 85(2), 151–164. Sheykhnazari, S., Tabarsa, T., Ashori, A., Shakeri, A., & Golalipour, M. (2011). Bacterial synthesized cellulose nanoﬁbers: Effects of growth times and culture mediums on the structural characteristics. Carbohydrate Polymers, 86(3), 1187–1191. Soykeabkaew, N., Arimoto, N., Nishino, T., & Peijs, T. (2008). All-cellulose composites by surface selective dissolution of aligned ligno-cellulosic ﬁbres. Composites Science and Technology, 68(10–11), 2201–2207. Sun, D., Yang, J., & Wang, X. (2010). Bacterial cellulose/TiO2 hybrid nanoﬁbers prepared by the surface hydrolysis method with molecular precision. Nanoscale, 2(2), 287–292.
Wan, Y. Z., Luo, H., He, F., Liang, H., Huang, Y., & Li, X. L. (2009). Mechanical, moisture absorption, and biodegradation behaviours of bacterial cellulose ﬁbrereinforced starch biocomposites. Composites Science and Technology, 69(7–8), 1212–1217. Xie, K., Yu, Y., & Shi, Y. (2009). Synthesis and characterization of cellulose/silica hybrid materials with chemical crosslinking. Carbohydrate Polymers, 78(4), 799–805. Xie, K., Zhang, Y., & Yu, Y. (2009). Preparation and characterization of cellulose hybrids grafted with the polyhedral oligomeric silsesquioxanes (POSS). Carbohydrate Polymers, 77(4), 858–862. Yano, H., Sugiyama, J., Nakagaito, A. N., Nogi, M., Matsuura, T., Hikita, M., et al. (2005). Optically transparent composites reinforced with networks of bacterial nanoﬁbers. Advanced Materials, 17(2), 153–155.